Nanotag luminescent fingerprint anti-counterfeiting technology
© Johansen et al.; licensee Springer. 2012
Received: 22 February 2012
Accepted: 22 May 2012
Published: 22 May 2012
We describe a method to fabricate, transfer and validate via image processing nanofibre-based, unique security marks (‘nanotags’) for anti-counterfeiting purposes. Epitaxial surface growth of oligophenylenes on a heated muscovite mica crystal results in a thin film of mutually aligned nanofibres with dimensions of tens of nanometres in height, hundreds of nanometres in width and tens to hundreds of micrometres in length. By applying a shadow mask, a film pattern is generated which contains only sparse, randomly grown nanofibres, which in turn represent a unique ‘fingerprint’ of the growth area. This fingerprint can be transferred on an adhesive tape as a label of a product, imaged using low magnification microscopy, digitalised and stored in a database. Infrared surface heating, enforced cooling and load lock transfer makes the fabrication process fast and scalable to mass production.
KeywordsAnti-counterfeit Organic nanofibres Molecular beam epitaxy Process optimisation
Counterfeiting is a steady and increasingly more important problem in all kind of commercialised production. Counterfeiting does not only inherently violate intellectual property rights of inventors and producers, but it also induces a real danger potential to customers, e.g. in the case of falsified drugs. A usual approach to anti-counterfeiting is to apply unique markers to the product in question. Unfortunately, readily available, advanced printing technologies provide simple access to high quality counterfeiting of such markers, especially those which are based on holographic patterns . Given this background, it is not surprising that a solution to this problem has to base on the introduction of new technologies which are more difficult to counterfeit. Bottom up nanotechnology is one of these more recent approaches, which can help addressing the problem since it per se can imply a stochastic generation of unique and irreproducible patterns of nanoscaled objects.
The principal problem with the use of bottom-up nanotechnology for the generation of unique anti-counterfeiting markers is the inherent optical invisibility of objects that are smaller than half the wavelength of the imaging light. Hence, the uniqueness of nanomarkers created by tailored nanoscaled objects becomes obvious only if one either employs state-of-the-art imaging technology (e.g. scanning electron or atomic force microscopy) or if one bases the detection on second-order effects, e.g. unique optical appearance as for quantum dots . For the purpose of anti-counterfeiting, it would, of course, be most interesting to have markers; the uniqueness of which can be detected on various identification levels, from bare eye over simple to advanced instrumentation.
A way to overcome this problem is to implement nanoscaled objects that possess a macroscopic dimension, e.g. 1D nanofibres, instead of quantum dots. In this work, we use luminescent markers generated by surface-grown patterns of organic nanofibres : these nanofibres exhibit bright, polarised and spatially strong anisotropic luminescence upon UV excitation  or current injection (L Tavares, J Kjelstrup-Hansen, and HG Rubahn, unpublished work), are visible by the naked eye since one of their dimensions is macroscopic and show unique patterns of mutually parallel-oriented entities under low magnification microscopy, which allows simple identification of individual tags made of these fibre arrays (HG Rubahn, S Johansen, and M Radziwon, unpublished work). The fibres are also chemically inert and withstand temperatures of more than 100°C. Ambient light does not cause photo-oxidation (‘bleaching’) of the nanofibres. However, strong UV excitation causes photobleaching and eventually destroys the fibres, but this process can be avoided by appropriate surface coating .
However, since the ordered molecular crystals from which these nanofibres are built are only weakly van der Waals bound; they are mechanically instable if released from the growth substrate, and thus, further manipulation (transfer  and integration) becomes extraordinarily difficult. A further challenge is large-scale production of nanofibre-based anti-counterfeit tags since the epitaxial growth state-of-the-art process of these nanoaggregates takes a significant amount of time - usually several hours.
In this present paper, we discuss results that show how to optimise organic nanofibre growth technology towards fast production (minutes rather than hours), how to make unique patterns easily identifiable using a shadow masking technology and how to integrate them into cheap and unique nanotags on adhesives.
The overall shape of the nanofibre tag as fabricated via vacuum deposition is governed by a round mask in front of the mica disc. The mask has a further shadowing cross in the middle, made of 300- to 700-mm-thick metal wires. On the mica substrate surface, the fibres form a densely packed layer of uniform thickness, which can be changed by varying the deposition rate and exposure time of the molecular beam. Due to the bright luminescence of p6P thin films, a mass thickness of 8 nm is sufficient for easy visibility of the fibre tag under LED UV illumination. The mass thickness is controlled by a quartz microbalance. In the shadowed area, the density of fibre growth is strongly decreased. However, fibres that started growing in the dense area extend into the shadowed regime, thus forming, via random growth, a unique nanofibre pattern.
Next, the as-grown fibres on the mica disc are covered by a transparent adhesive tape, which not only does not significantly affect the blue emission of the fibres, but also serves as a protective cover. By peeling off the tape from the substrate, the mica disc supporting the fibres is cleaved to an ultrathin and transparent layer. Hence, the fibres on the ultrathin mica disc are surrounded by an adhesive area and can be directly mounted on the product to be marked. By shaping the shadow mask in a unidirectional manner, a fiducial point on the surface of the tag can always be identified in a low magnification microscopic image of the surface; the unique nanofibre pattern can thus be detected and extracted by an image processing software.
Results and discussion
It is well known that p6P nanofibre growth on mica occurs in several steps: first, a wetting layer of molecules is formed on the substrate, followed by the formation of small clusters. Due to the surface temperature, these clusters are mobile and form aggregates. Since p6P is a rod-like molecule, the aggregates grow via side-to-side attachment of molecules, which limits the growth to one dimension on the surface. Due to the mobility of molecules and clusters on the surface of the aggregates, growth normal to the surface is also hindered. As a result, fibre-like structures with well-defined molecular order are formed. The orientation of the fibres is given by the orientation of the molecules, and this in turn is dictated by growth epitaxy . Due to this characteristic growth process, the mica-grown nanofibres are always mutually aligned, but the individual pattern is not reproducible.
The processed image consists of two types of lines: baselines being the borders of the masked region and lines corresponding to fibres which have grown underneath the mask. The angles at which those fibres grow, and especially the coordinates of their terminators, are stochastic parameters. Therefore, this information derived from the image is truly unique for each sample.
Distinction between two coordinate matrices of different samples relies therefore on the ability to position the fibre in relation to the border of the masked region. Due to the implemented image processing sequence, the fibre needs to have at least a 4-pixel width to be detected, and the minimum distance between fibres is 8 pixels. This limits the average number of detectable fibre terminations on the borderline to √2/8 × the image width which, for exemplary images, equals to 110. If we want to detect only the 10 most distinct fibres, it gives over 4 × 1013 combinations (10 out of 110) of fibre starting points solely. In addition, this number will increase by a factor of about 103 due to variations in the fibre tilt angles. Therefore, the parameter variation is large enough for most counterfeit applications.
After fabrication and UV-assisted optical inspection of each produced marker, its coordinate matrix is stored in a secured database, paired with information on the particular tag (serial number, production date etc.). When a product is marked with a tag, it can always be determined whether it is genuine by taking a low magnification UV-exposed microscopic photograph of the tag and extracting the fingerprint data to compare it with that already existing in the database.
In this article, we have presented a method to generate unique nanotags for product anti-counterfeiting using bottom-up grown arrays of ordered organic nanofibres. The resulting nanotags can be readily transferred onto arbitrary products using transparent adhesive foils. Due to the simplicity of fibre array generation, there is no principal obstacle for upscaling the method to large-scale production.
atomic force microscopy
We are grateful to the proof-of-concept scheme of Danish Agency for Science, Technology and Innovation for supporting this work.
- van Renesse R: A review of holograms and other microstructures as security features in the holography. In The First 50 Years Springer Series in Optical Sciences. Edited by: Fournier JM. Springer-Verlag Berlin and Heidelberg GmbH & Co. K, Berlin; 2003:78.Google Scholar
- Brien PO, Pickett N: Strategies for the scalable synthesis of quantum dots and related nanodimensional materials, in the chemistry of nanomaterials. In Synthesis, Properties and Applications. Edited by: Rao CNR, Müller A, Cheetham AK. Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim; 2005:12–30.Google Scholar
- Balzer F, Rubahn HG: Dipole-assisted self-assembly of light-emitting p-nP needles on mica. Appl Phys Lett 2001, 79: 3860–3862. 10.1063/1.1424071View ArticleGoogle Scholar
- Balzer F, Rubahn HG: Growth control and optics of organic nanoaggregates. Adv Funct Mater 2005, 15: 17–24. 10.1002/adfm.200400367View ArticleGoogle Scholar
- Tavares L, Kjelstrup-Hansen J, Sturm H, Rubahn HG: Reduced bleaching in organic nanofibers by bi-layer polymer/oxide coating. J Appl Phys 2010, 107: 103521. 10.1063/1.3427561View ArticleGoogle Scholar
- Balzer F, Rubahn HG: Soft lift-off of organic nanofibers. European Pat Appl Publication 2011, 1: 812–978.Google Scholar
- Brewer J, Maibohm C, Jozefowski L, Bagatolli L, Rubahn HG: A 3D view on free floating, space fixed and surface bound para-phenylene nanofibers. Nanotechnology 2005, 16: 2396–2401. 10.1088/0957-4484/16/10/067View ArticleGoogle Scholar
- Balzer F, Pogantsch A, Rubahn HG: Temperature dependent analysis of three classes of fluorescence spectra from p6P nanofiber films J. Lumin 2009, 129: 784–789. 10.1016/j.jlumin.2009.02.014View ArticleGoogle Scholar
- Kankate L, Balzer F, Niehus H, Rubahn HG: From clusters to fibers: parameters for discontinuous p-6P thin film growth J. Chem Phys 2008, 128: 084709.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.